**Theory of Conductivity in Semiconducting Single-Wall **

**Carbon Nanotubes **

**Shigeji Fujita1, Salvador Godoy2, Akira Suzuki3***
1_{Department of Physics, University at Buffalo, Buffalo, USA }

2_{Departamento de Física, Facultad de Ciencias, Universidad Nacional Autónoma de México, Mexico City, Mexico }
3_{Department of Physics, Faculty of Science, Tokyo University of Science, Shinjuku-ku, Japan }

Email: *_{asuzuki@rs.kagu.tus.ac.jp }

Received August 13, 2012; revised September 16, 2012; accepted September 23,2012

**ABSTRACT **

The conduction of a single-wall carbon nanotube depends on the pitch. If there are an integral number of carbon hexa-gons per pitch, then the system is periodic along the tube axis and allows “holes” (not “electrons”) to move inside the tube. This case accounts for a semiconducting behavior with the activation energy of the order of around 3 meV. There is a distribution of the activation energy since the pitch and the circumference can vary. Otherwise nanotubes show me-tallic behaviors (significantly higher conductivity). “Electrons” and “holes” can move in the graphene wall (two dimen-sions). The conduction in the wall is the same as in graphene if the finiteness of the circumference is disregarded. Coo-per pairs formed by the phonon exchange attraction moving in the wall is shown to generate a temCoo-perature-independent conduction at low temperature (3 - 20 K).

**Keywords:** Semiconducting SWNT; Cartesian Unit Cell Model; Cooper Pair; Bloch Electron Dynamics

**1. Introduction **

Iijima [1] found after his electron diffraction analysis
that carbon nanotubes ranging 4 to 30 nanometers (nm)
in diameter have helical multi-walled structures. Single-
wall nanotube (SWNT) has about one nanometer in
di-ameter and micrometers (μm) in length. Ebbesen *et al.* [2]

measured the electrical conductivity of individual
carbon nanotubes and found that varies depending of
the temperature *T*, the tube radius *r* and the pitch *p*.

Ex-periments show that SWNT can be either semiconducting
or metallic, depending on how they are rolled up from
the graphene sheets [3]. In the present work we shall
present a microscopic theory of the electrical
conductiv-ity of semiconducting SWNT, starting with a graphene
honeycomb lattice, developing a Bloch electron
dynam-ics based on a rectangular cell model [4], and using
ki-netic theory. A SWNT can be formed by rolling a
gra-phene sheet into a circular cylinder. The gragra-phene which
forms a honeycomb lattice is intrinsically anisotropic as
we shall explain it in more detail later in Section 2.
Mo-riyama *et al.* [5] fabricated 12 SWNT devices from one

chip, and observed that two of the SWNT samples are semiconducting and the other 10 are metallic. The semi-conducting SWNT samples show an activated-state

tem-perature behavior. That is, the resistance decreases with increasing temperature. Why are there two sets of sam-ples showing very different behavior? The answer to this question is as follows.

The line passing the centers of the nearest-neighbor
carbon hexagons forms a helical line around the
nano-tube with a pitch *p* and a radius *r*.

In **Figure 1(a)**, a section of the circular tube with a

pitch *p* is drawn. Its unrolled plane is shown in **(b)**. The

circumference likely contains an integral number

*m* of the carbon hexagons (units). The pitch *p*, however,

may or may not contain an integral number* n* of units. In

the fabrication process the pitch is not controlled. In the first alternative, the nanotube is periodic with the period

*p* along the tube axis. Then, there is a one-dimensional

(1D) *k*-vector along the tube. A “hole” which has a

posi-tive charge +*e* and a size of a unit ring of height *p* and

radius *r* can go through inside the positively charged

carbon wall. An “electron” having a negative charge −*e*

and a similar size is attracted by the carbon wall, and
hence it cannot go straight inside the wall. Thus, there
should be an extra “hole” channel current in a SWNT.
Moriyama* et al. *[5] observed a “hole”-like current after

examining the gate voltage effect. The system should have the lowest energy if the unit ring contains an integer set

2π*r*

(a) (b)

**Figure 1. (a) A section circular tube wall with a radius r and ****a pith p; (b) Its unrolled plane. **

after annealing at high temperatures. This should happen if the tube length is comparable with the circumference. The experimental tube length is much greater than the circumference, and the pitch angle can be varied con-tinuously. The set of irrational numbers is greater in car-dinality than the set of rational numbers. Then, the first case in which the unit contains an integer set

###

*m n*,

###

ofhexagons must be the minority. This case then generates a semiconducting transport behavior. We shall show later that the transport requires an activation energy. Fujita and Suzuki [4] showed that the “electrons” and “holes” must be activated based on the rectangular unit cell mod-el for graphene.

Saito, Dresselhaus and Dresselhaus [3] state that a SWNT is characterized by two integer indices

###

*m n*,

###

*m**n*

ˆ ˆ ˆ ,

, for example, for an armchair nanotube whereas

for a zigzag nanotube. If is a multiple of 3, then a SWNT is metallic. They then argued that ap-proximately one third of the SWNT are metallic, and the other two thirds are semiconducting. This model is in variance with the experimental observation by Moriyama

*et al. *[5], where the majority of SWNT is metallic. We

must look for a different classification scheme.

0

*m* *n m*

If a SWNT contains an irrational number of carbon hexagons, which happens more often, then the system does not allow a conduction along the tube axis. The system is still conductive since the conduction electrons (“electrons”, “holes”) can go through in the tube wall. This conduction is two-dimensional (2D), opposed to 1D, as can be seen in the unrolled configuration, which is precisely the graphene honeycomb lattice. This means that the conduction in the carbon wall should be the same as the conduction in graphene if the effect of the finite-ness of the radius is neglected.

We consider graphene in Section 2. The current band theory of the honeycomb crystal is based on the Wigner- Seitz (WS) cell model [3,6]. The model applied to gra-phene predict a gapless semiconductor, which is not

ob-served. The WS model [6] is suitable for the study of the ground-state energy of the crystal. To describe the Bloch electron dynamics [7] a new theory based on the Carte-sian unit cell not matching with the natural triangular crystal axes must be used. Also the phonons can be dis-cussed using Cartesian coordinate-systems, not with the triangular coordinate-systems. The conduction electron moves as a wave packet formed by the Bloch waves as pointed out by Ashcroft and Mermin in their book [7]. This picture is fully incorporated in our new theoretical model.

**2. Graphene **

We consider a graphene, in which carbon ions (C+_{) }
oc-cupy a 2D honeycomb lattice, See **Figure 2**. The normal

current carriers are “electrons” and “holes”. Following
Ashcroft and Mermin [7], we adopt the semiclassical
model of electron dynamics in solids. “Electrons”
(“holes”) are defined as quasi-electrons which move
counterclockwise (clockwise) viewed from the tip of the
applied magnetic field. In the semiclassical (wave packet)
theory, it is necessary to introduce a * k*-vector:

*x* *x* *y* *y* *z* *z*

**k****k e****k e****k e**

ˆ

(1)

where * ex*,

*ˆ*

**e***y*,

*ˆ*

**e***z*are the Cartesian orthonormal vec-

tors, since the * k*-vectors are involved in the semi-

classical equation of motion:

###

###

d

,

d*t* *q*

* k*

* k*

**E**

**v B**

*q*

(2)

where is the charge of a conduction electron, and * E*
and are the electric and magnetic fields, respectively.
The vector

**B**

1

**v****k**

###

=

**k**

*z*

(3)

is the electron velocity, where is the energy. The 2D crystals such as graphene can also be treated similarly, only the -component being dropped. The choice of the Cartesian axes and the unit cell is obvious for the cubic crystals. We must choose an orthogonal unit cell also for the honeycomb lattice, as demonstrated below.

Graphene forms a 2D honeycomb lattice. The WS unit
cell is a rhombus shown in **Figure 2(a)**.

###

*V* * r* is lattice-periodic:
The potential energy

###

*mn*

###

###

,*V* * r*

**

**R***V*

**r**1 2,

*mn* *m* *n*

(4)

where

**R****a*** a* (5)

###

is a Bravais vector with the primitive vectors

**a a**_{1},

_{2}

###

and integers

###

*m n*,

###

**r**

,
*mn*

**r****r*** R*

**r**

(6)
where is the point defined within the standard unit
cell. Equation (4) describes the 2D lattice periodicity
but does* not* establish the * k*-space, which is explained

below.

To see this clearly, we first consider an electron in a simple square (sq) lattice. The Schrödingier wave equa-tion is

###

2 2###

*i sq

###

2 *V*

*t* *m*

_{ } _{} _{}

**r****r****r****r**

0

*mn*

**R**

ˆ ˆ ,

nstant)

*x* *y*

*ma* *na*

* e*

**e**

##

0##

###

sq

*mn* *V*

**r**

. (7)

The Bravais vector for the sq lattice is 0

( lattice co

*mn* *x* *y*

*a*
* R*

*m*

**a***n*

**a**(8)

The system is lattice periodic:

sq

*V* **r*** R* . (9)

If we choose a set of Cartesian coordinates

###

*x y*,

along the sq lattice, then the Laplacian term in Equation (7) is given by

###

22 22###

, .2 _{,}

*x y* *x y*

*x* *y*

_{}

###

*V*

**r**

_{ }

(10)

If we choose a periodic square boundary with the side
length *Na*, *N* = integer, then there are 2D Fourier

trans-forms and * k*-vectors.

We now go back to the original graphene system. If
we choose the *x*-axis along either * a*1 or

*2, then the*

**a**po-tential energy field is periodic in the *x*-direction

but it is aperiodic in the *y*-direction. For an infinite lattice

the periodic boundary is the only acceptable boundary
condition for the Fourier transformation. Then, there is
no 2D * k*-space spanned by 2D

*-vectors. If we omit the*

**k**kinetic energy term, then we can still use Equation (4) and obtain the ground state energy (except the zero point energy).

We now choose the orthogonal unit cell shown in **Fig- **
**ure 2(b)**. The unit has side lengths

1 3 ,0 2 3 ,0

*b* *a* *b* *a*

*a*

(11)
where 0 is the nearest neighbor distance between two
C’s. The unit cell has four (4) C’s. The system is lattice-
periodic in the *x*- and *y*-directions, and hence there are

2D *k*-space.

The “electron” (“hole”) is defined as a *quasi-electron *

which has an energy higher (lower) than the Fermi
en-ergy *F* and “electron” (“hole”) are excited on the

posi-tive (negaposi-tive) side of the Fermi surface with the conven-tion that the positive normal vector at the surface points in the energy-increasing direction.

The “electron” (wave packet) may move up or down
along the *y*-axis to the neighboring unit cells passing

(a) (b)

**Figure 2. (a) WS unit cell, rhombus (dotted lines) for **
**gra-phene; (b) The orthogonal unit cell, rectangle (dotted lines). **

over one C+_{. The positively charged C}+_{ acts as a }
wel-coming (favorable) potential valley for the negatively
charged “electron”, while the same C+_{ act as a hindering }
potential hill for the positively charged “hole”. The
“hole”, however, can move horizontally along the *x*-axis

without meeting the hindering potential hills. Thus the
easy channel directions for the “elections” (“holes”) are
along the *y*- (*x*-) axes.

Let us consider the system (graphene) at 0 K. If we put
an electron in the crystal, then the electron should occupy
the center O of the Brillouin zone, where the lowest
en-ergy lies. Additional electrons occupy points neighboring
the center O in consideration of Pauli’s exclusion
princi-ple. The electron distribution is *lattice-periodic* over the

entire crystal in accordance with the Bloch theorem [8].
Carbon (C) is a quadrivalent metal. The first few low-
lying energy bands are completely filled. The uppermost
partially filled bands are important for transport
proper-ties discussion. We consider such a band. The (2D)
Fer-mi surface, which defines the boundary between the
filled and unfilled * k*-space (area) is not a circle since the

*x-y* symmetry is broken (*b**c*). The “electron” effective
mass is lighter in the direction [110] than perpendicular
to it. Hence the electron motion is *intrinsically *
*anisot-ropic*. The negatively charged “electron” is near the

posi-tive ions C+_{. Hence, the gain in the Colulomb interaction }
is greater for “electron”. Thus, the “electrons” are the
majority carriers at zero gate voltage. That is, the system
has two different masses and it is intrinsically anisotropic.
If the electron number is raised by the gate voltage
ap-plied perpendicular to the plane, then the Fermi surface
more quickly grows in the easy-axis (*y*-) direction than in

the *x*-direction. The Fermi surface must approach the

Brillouin boundary at right angles because of the inver-sion symmetry possessed by honeycomb lattice [9]. Then at a certain voltage, a “neck” Fermi surface must be de-veloped.

[image:3.595.333.507.82.202.2]current (magnitude) along the field direction is pro-portional to [10]

###

###

###

###

###

###

2

channels

2 2 2

cos ,

cos cos 2π3 cos 2π3 3 2.

###

(12)

E 3 meV Note that this current does not depend on the angle

between the field direction () and the channel current direction ( ). More detailed discussion can be found in ref. [10]. Hence, the graphene does not show anisotropy in the conductivity.

1< 2

We have seen earlier that the “electron” and “hole” have different internal charge distributions and therefore have different effective masses. Which carriers are easier to be activated or excited? The “electron” is near the pos-itive ions and the “hole” is farther away from the ions. Hence, the gain in the Coulomb interaction is greater for the “electron”. That is, the “electrons” are more easily activated (or excited). The presence of the welcoming C+ ions in the channel direction also enhances this inequal-ity.

We may represent the activation energy difference by [6]

.

(13) The thermally-activated (or excited) electron densities are given by

###

p###

*j*

*k T*B

###

,= 1

*j*

ex

*j* *j*

*n T* *n* (14)

where and 2 represent the “electron” and “hole”,
respectively. The prefactor *nj* is the density at high-

temperature limit.

**3. SWNT **

Let us consider the long SWNT rolled with a graphene
sheet. The charge may be transported by the channeling
“electrons” and “holes” in the graphene wall. But the
“holes” within the wall can also contribute to the charge
transport. Because of this extra channel inside the carbon
nanotube, “holes” are likely to be the majority carriers in
nanotubes although “electrons” are the dominant carriers
in graphene. Moriyama *et al.* [5] studied the electrical

transport in semiconducting SWNT in the temperature
range 2.6 - 200 K, and found from the filed (gate voltage)
effect that the carriers are “hole”-like. Their data are re-
produced in **Figure 3**.

The conductivity depends on the pitch of the SWNT.
The helical line is defined as the line passing the nearest
neighbors of the C-hexagons. The helical angle is the
angle between the helical line and the tube axis. The
degree of helicity *h* may be defined as

cos .

*h* (15)

For a macroscopically large graphene the conductivity

**Figure 3. Log-scale plot of the currents in semiconducting **
**SWNT as a function of inverse temperature after **
**Mori-yama et al. [5]. **

is isotropic as we saw in Section 2. The conductivity in (semiconducting) SWNT depends on this helicity . This is a kind of a finite size effect. The circumference is finite while the tube length is macroscopic.

*h*

In a four-valance-electron conductor such as graphene
all electrons are bound to ions at 0 K, and there is no
conduction. If a “hole” having the charge +*e* and the size

of a unit ring is excited, then this “hole” can move along
the tube axis with the activation energy 3 and the
ef-fective mass *m*3. Both 3 and depend on the
ra-dius and the pitch. 3

*m*

*m*

We are now ready to discuss the conductivity of se-miconducting SWNT. There are four currents carried by

1) “Electrons” moving in the graphene wall with the
mass 1 and the density *n*1exp

###

1*k T*B

###

, running inthe channels 110 .

*m*

2) “Holes” moving in the graphene wall with the mass
2 and the density *n*2exp

###

2*k T*B

###

, running in thechannels 100

*m*

.

3) “Holes” moving with the mass 3 and the density

###

###

exp

*n*3 3 *k T*B , running in the tube-axis direction. The

activation (or excitation) energy 3 and the effective mass 3 vary with the radius and the pitch.

4) Cooper pairs (pairons) formed by the phonon- exchange attraction, which move in the graphene wall.

*m*

In actuality, one of the currents may be dominant, and be observed.

In the normal Ohmic conduction due to the conduction electrons the resistance is proportional to the sample (tube) length. Then, the conductivity is given by the Drude formula:

2 2

* *

1 ,

*nq* *nq*
*m* *m*

###

_{,}*

*e* *m*

(16)

mass, *n* the carrier density, and the relaxation

(colli-sion) time. The relaxation rate _{Γ}_{}_{}1

Γ

###

ph *T* .

Γ

is the inverse of the relaxation time. If the impurities and phonons are scatterers, then the rate is the sum of the impurity scattering rate and the phonon scattering rate

: imp imp

###

ph*T*(17)

The impurity scattering rate imp is temperature- independent and the phonon scattering rate Γ

###

*T*

###

*T*

###

above 2 K###

Γ

ph is

temperature -dependent. The phonon scattering rate is linear in

###

*T*above around 2 K:

*T* *a* *a*

###

###

ph*T*

###

ph*T*Γ

###

phΓ *T*, constant,

###

*n T*

. (18)
The temperature dependence should arise from the
carrier density and the phonon scattering rate
. Writing the *T*-dependence explicitly, we obtain

from Equations (14)-(18)

2

*

= e B

imp
1
Γ
*k T*
*j*
*j*
*j*
*n*
*aT*

3 3 meV

. (19)

*j*

*e*

*m*

###

Moriyama *et al.* [5] used the Arrhenius plot for the

data above 20 K and obtained the activation energy

.

*n*

(20) By studying the field (gate voltage) effect, the carriers were found to be “hole”-like. Thus, the major currents observed can be interpreted in terms of the “holes” mov-ing within the tube wall.

This “hole” axial transport depends on the unit ring
containing hexagons. Since the pitch and the
cir-cumference have distributions, the activation energy *m* _{3}
should also have a distribution. Hence the obtained value
in Equation (20) must be regarded as the averaged value.

Liu *et al. *[10] systematically measured the resistance

of SWNT under hydrostatic pressures, and fitted
their data by using 2D *variable range hopping* (vrh)

theoretical formula [11]:

###

*T*

###

###

###

1 3 0exp*T T*0 ,

0 525 K

*T*

*T*

(21)

where

(22) is a fit (temperature) parameter and 0 a (resistance) parameter. Mott’s vrh theory [12] is applicable when highly random disorders exist in the system. An individ-ual SWNT (annealed) is unlikely to have such random-ness. We take a different view here. The scatterings are due to impurities and phonons. But carriers (“holes”) have a distribution in the unit cell size. Hence the distri-bution of the activation energy introduces the flattening of the Arrhenius slope by the factor 1/3. Compare Equa-tion (21) and EquaEqua-tion (14).

The “hole” size is much greater than the usually

as-sumed atomic impurity size and the phonon size, which
are of the order of the lattice constant. This size mismatch
may account for a ballistic charge transport observed by
Frank *et al*. [13] and others [14]. More careful studies are

required to establish the cause of the ballisticity.

We now go back to the data shown in **Figure 3**. Below

20 K the currents observed are very small and they ap-pear to approach a constant in the low temperature limit (large 1

*T* limit). These currents, we believe, are due to
the Cooper pairs.

The Cooper pairs (pairons) move in 2D with the linear dispersion relation [15]:

*j* _{,}

*c* *p*
(23)

###

F 2 π ,*j* *j*

*c* *v*

(24)
where _{F}*j*

*v* is the Fermi velocity of the “electron” (*j* = 1)

[“hole” (*j* = 2)].

Consider first “electron”-pairs. The velocity * v* is given

by (omitting superscript)

or *x*,

*x*

*x*

*p*
*p*

*v* *c*

*p p* *p*

**v**

* p* (25)

where

2 2_{.}

*x* *y*

*p* *p* *p* (26)

The equation of motion along the * E*-field (

*x*-) di-

rection is
,
*x*
*p*
*q E*
*t*
_{} _{}
*q*
(27)

is the charge 2*e*

where of a pairon. The solution of Equation (27) is given by

0_{,}

*x* *x*

*p* *q Et* *p*
0

(28)
where *px* is the initial momentum component. The

current density *j*p is calculated from (charge *q*) ×
(number density *n*p) × (average velocity * v* ). The
av-erage velocity

*is calculated by using Equations (25) and (28) with the assumption that the pair is accelerated only for the collision time . We then obtain*

**v**###

###

2p p p p

1 *c* _{.}

*j* *q n v* *q n c* *q E* *q* *n E*

*p* *p*

###

(29)

For stationary currents, the pairon density *n*p is given

by the Bose distribution function *f* * _{p}* :

###

###

###

1p *p* exp *p* B 1 ,

*n* *f* _{} *k T* _{} (30)

*e* is the fugacity. Integrating the current _{p}

where *j*

*p* *j* *E*

over all 2D -space, and using Ohm’s law we obtain for the conductivity :

###

_{2}

_{π}

###

2 2_{d}2 1

###

_{.}

*p*

*q c* *pp f*

_{}

###

In the temperature ranging between 2 and 20 K we may assume the Boltzmann distribution function for

*p*

*f* :

###

*p*exp

###

*p*B

###

.*f* *k T*

###

1 =*aT*

*p*

(32)

We assume that the relaxation time arises from the phonon scattering so that , see Equations (16)-(18). After performing the -integration we obtain

2 B 2 2

, π

*e k*
*e*
*a*

(33) which is temperature-independent. If there are “elec-trons” and “hole” pairs, they contribute additively to the conductivity. These pairons should undergo a Bose-Ein- stein condensation at a temperature lower than 2.2 K. We predict a superconducting state at lower temperatures.

**4. Summary and Discussion **

A SWNT is likely to have an integral number of carbon
hexagons around the circumference. If each pitch
con-tains an integral number of hexagons, then the system is
periodic along the tube axis, and “holes” (and not
“elec-trons”) can move along the tube axis. The system is
se-miconducting with an activation energy _{3}. This energy

3

has a distribution since both pitch and circumference have distributions. The pitch angle is not controlled in the fabrication processes. There are more numerous cases where the pitch contains an irrational numbers of hexa-gons. In these cases the system shows a metallic behavior experimentally [16].

In the process of arriving at our main conclusion we have uncovered the following results.

1) “Electrons” and “holes” can move in 2D in the car-bon wall in the same manner as in graphene.

2) For a metallic SWNT 1) implies that the conduction in the wall shows no pitch dependence.

3) The Cooper pairs are formed in the wall. They should undergo Bose-Einstein condensation at lower temperature, exhibiting a superconducting state.

A metallic SWNT will be treated separately.

**REFERENCES **

[1] S. Iijima, “Helical Microtubules of Graphitic Carbon,”

*Nature*, Vol. 354, 1991, pp. 56-58. doi:10.1038/354056a0

[2] T. W. Ebbesen, H. J. Lezec, H. Hiura, J. W. Bennet , H. F.
Ghaemi and T. Thio, “Electrical Conductivity of
Individ-ual Carbon Nanotubes,” *Nature*, Vol. 382, 1996, pp. 54-

56. doi:10.1038/382054a0

[3] R. Saito, G. Dresselhaus and M. S. Dresselhaus, “Physi- cal Properties of Carbon Nanotubes,” Imperial College Press, London, 1998, pp. 35-58.

doi:10.1142/9781860943799_0003

[4] S. Fujita and A. Suzuki, “Theory of Temperature De-pendence of the Conductivity in Carbon Nanotubes,”

*Journal of Applied Physics*, Vol. 107, 2010, Article ID:

013711. doi:10.1063/1.3280035

[5] S. Moriyama, K. Toratani, D. Tsuya, M. Suzuki, Y.
Ao-yagi and K. Ishibashi, “Electrical Transport in
Semicon-ducting Carbon Nanotubes,”* Physica E*, Vol. 24, No. 1-2,

2004, pp. 46-49. doi:10.1016/j.physe.2004.04.022 [6] E. Wigner and F. Seitz, “On the Constitution of Metallic

Sodium,”* Physical Review*, Vol. 43, No. 10, 1933, pp.

804-810. doi:10.1103/PhysRev.43.804

[7] N. W. Ashcroft and N. D. Mermin, “Solid State Physics,” Saunders, 1976, pp. 91-93, 217, 228, 229.

[8] F. Bloch, “Über die Quantenmechanik der Elektronen in
Kristallgittern,”* Zeit Physik*, Vol. 52, 1928, pp. 555-599.

[9] S. Fujita and K. Ito, “Quantum Theory of Conducting Matter,” Springer, New York, 2007, pp. 85-90,106-107. doi:10.1007/978-0-387-74103-1

[10] S. Fujita, A. Garcia, D. O’Leyar, S. Watanabe and T.
Burnett, “On the Conductance of a Lattice-Like Net-
work,”* Journal of Physics and Chemistry of Solids*, Vol.

50, No. 1, 1989, pp. 27-31.

doi:10.1016/0022-3697(89)90468-X

[11] B. Liu, B. Sundqvist, O. Andersson, T. Wågberg, E. B.
Nyeanchi, X.-M. Zhu and G. Zou, “Electric Resistance of
Single-Walled Carbon Nanotubes under Hydrostatic
Pressure,” *Solid State Communications*, Vol. 118, No. 1,

2001, pp. 31-36. doi:10.1016/S0038-1098(01)00034-5 [12] N. F. Mott, “Conduction in Non-Crystalline Materials,”

Oxford University Press, Oxford, 1987.

[13] S. Frank, P. Poncharal, Z. I. Wang and W. A. de Heer,
“Carbon Nanotube Quantum Resistors,”* Science*, Vol.

280, No. 5370, 1998, pp. 1744-1746. doi:10.1126/science.280.5370.1744

[14] A. Javey, J. Guo, Q. Wang, M. Lundstrom and H. Dai, “Ballistic Carbon Nanotube Field-Effect Transistors,”

*Nature*, Vol. 424, 2003, pp. 654-657.

doi:10.1038/nature01797

[15] S. Fujita, K. Ito and S. Godoy, “Quantum Theory of Conducting Matter: Superconductivity,” Springer, New York, 2009, pp. 77-79.

[16] S. J. Tans, M. H. Devoret, H. Dai, A. Thess, R. E.
Smal-ley, L. J. Geerligs and C. Dekker, “Individual Single-Wall
Carbon Nanotubes as Quantum Wires,”* Nature*, Vol. 386,